General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.9 - 7.92 g/cm³ Show Material materials with Density of 7.9 - 7.92 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -269.0 °C | 201.3 GPa Show Material materials with Elastic modulus of 201.3 GPa |

-195.0 °C | 205.1 GPa Show Material materials with Elastic modulus of 205.1 GPa | |

-100.0 °C | 206 GPa Show Material materials with Elastic modulus of 206 GPa | |

20.0 °C | 196 - 200 GPa Show Material materials with Elastic modulus of 196 - 200 GPa | |

27.0 °C | 190.2 GPa Show Material materials with Elastic modulus of 190.2 GPa | |

100.0 °C | 190 - 194 GPa Show Material materials with Elastic modulus of 190 - 194 GPa | |

200.0 °C | 182 - 186 GPa Show Material materials with Elastic modulus of 182 - 186 GPa | |

300.0 °C | 174 - 179 GPa Show Material materials with Elastic modulus of 174 - 179 GPa | |

400.0 °C | 166 - 172 GPa Show Material materials with Elastic modulus of 166 - 172 GPa | |

500.0 °C | 158 - 165 GPa Show Material materials with Elastic modulus of 158 - 165 GPa | |

600.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | |

700.0 °C | 142 GPa Show Material materials with Elastic modulus of 142 GPa | |

800.0 °C | 134 GPa Show Material materials with Elastic modulus of 134 GPa | |

Elongation | 20.0 °C | 45 % Show Material materials with Elongation of 45 % |

Elongation A80 | 20.0 °C | 45 % Show Material materials with Elongation A80 of 45 % |

Elongation A80, transverse | 20.0 °C | 45 % Show Material materials with Elongation A80, transverse of 45 % |

Elongation, transverse | 20.0 °C | 45 % Show Material materials with Elongation, transverse of 45 % |

Poisson's ratio | -269.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] |

-195.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

20.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

27.0 °C | 0.27 [-] Show Material materials with Poisson's ratio of 0.27 [-] | |

Unlock all property charts | ||

Shear modulus | 20.0 °C | 75.7 GPa Show Material materials with Shear modulus of 75.7 GPa |

Tensile strength | 20.0 °C | 500 - 700 MPa Show Material materials with Tensile strength of 500 - 700 MPa |

50.0 °C | 466 MPa Show Material materials with Tensile strength of 466 MPa | |

100.0 °C | 410 MPa Show Material materials with Tensile strength of 410 MPa | |

150.0 °C | 380 MPa Show Material materials with Tensile strength of 380 MPa | |

200.0 °C | 360 MPa Show Material materials with Tensile strength of 360 MPa | |

250.0 °C | 350 MPa Show Material materials with Tensile strength of 350 MPa | |

300.0 °C | 340 MPa Show Material materials with Tensile strength of 340 MPa | |

350.0 °C | 340 MPa Show Material materials with Tensile strength of 340 MPa | |

Unlock all property charts | ||

Tensile strength, transverse | 20.0 °C | 500 - 700 MPa Show Material materials with Tensile strength, transverse of 500 - 700 MPa |

Yield strength Rp0.2 | 20.0 °C | 200 MPa Show Material materials with Yield strength Rp0.2 of 200 MPa |

50.0 °C | 180 MPa Show Material materials with Yield strength Rp0.2 of 180 MPa | |

100.0 °C | 147 MPa Show Material materials with Yield strength Rp0.2 of 147 MPa | |

150.0 °C | 132 MPa Show Material materials with Yield strength Rp0.2 of 132 MPa | |

200.0 °C | 118 MPa Show Material materials with Yield strength Rp0.2 of 118 MPa | |

250.0 °C | 108 MPa Show Material materials with Yield strength Rp0.2 of 108 MPa | |

300.0 °C | 100 MPa Show Material materials with Yield strength Rp0.2 of 100 MPa | |

350.0 °C | 94 MPa Show Material materials with Yield strength Rp0.2 of 94 MPa | |

400.0 °C | 89 MPa Show Material materials with Yield strength Rp0.2 of 89 MPa | |

450.0 °C | 85 MPa Show Material materials with Yield strength Rp0.2 of 85 MPa | |

500.0 °C | 81 MPa Show Material materials with Yield strength Rp0.2 of 81 MPa | |

550.0 °C | 80 MPa Show Material materials with Yield strength Rp0.2 of 80 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2, transverse | 20.0 °C | 200 - 220 MPa Show Material materials with Yield strength Rp0.2, transverse of 200 - 220 MPa |

Yield strength Rp1.0 | 20.0 °C | 240 - 250 MPa Show Material materials with Yield strength Rp1.0 of 240 - 250 MPa |

50.0 °C | 218 MPa Show Material materials with Yield strength Rp1.0 of 218 MPa | |

100.0 °C | 181 MPa Show Material materials with Yield strength Rp1.0 of 181 MPa | |

150.0 °C | 162 MPa Show Material materials with Yield strength Rp1.0 of 162 MPa | |

200.0 °C | 147 MPa Show Material materials with Yield strength Rp1.0 of 147 MPa | |

250.0 °C | 137 MPa Show Material materials with Yield strength Rp1.0 of 137 MPa | |

300.0 °C | 127 MPa Show Material materials with Yield strength Rp1.0 of 127 MPa | |

350.0 °C | 121 MPa Show Material materials with Yield strength Rp1.0 of 121 MPa | |

400.0 °C | 116 MPa Show Material materials with Yield strength Rp1.0 of 116 MPa | |

450.0 °C | 112 MPa Show Material materials with Yield strength Rp1.0 of 112 MPa | |

500.0 °C | 109 MPa Show Material materials with Yield strength Rp1.0 of 109 MPa | |

550.0 °C | 108 MPa Show Material materials with Yield strength Rp1.0 of 108 MPa | |

Unlock all property charts | ||

Yield strength Rp1.0, transverse | 20.0 °C | 240 - 250 MPa Show Material materials with Yield strength Rp1.0, transverse of 240 - 250 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | |

20.0 °C | 1.61E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 1/K | ||

100.0 °C | 1.6E-5 - 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.6E-5 - 1.67E-5 1/K | ||

200.0 °C | 1.65E-5 - 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.65E-5 - 1.72E-5 1/K | ||

300.0 °C | 1.7E-5 - 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.7E-5 - 1.77E-5 1/K | ||

400.0 °C | 1.75E-5 - 1.81E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.75E-5 - 1.81E-5 1/K | ||

500.0 °C | 1.8E-5 - 1.84E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.8E-5 - 1.84E-5 1/K | ||

600.0 °C | 1.88E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.88E-5 1/K | ||

700.0 °C | 1.91E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.91E-5 1/K | ||

800.0 °C | 1.94E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.94E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 0 - 300 °C Show Material materials with Max service temperature, long of 0 - 300 °C | ||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | -100.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

20.0 °C | 472 - 500 J/(kg·K) Show Material materials with Specific heat capacity of 472 - 500 J/(kg·K) | ||

100.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

200.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

300.0 °C | 512 J/(kg·K) Show Material materials with Specific heat capacity of 512 J/(kg·K) | ||

400.0 °C | 520 J/(kg·K) Show Material materials with Specific heat capacity of 520 J/(kg·K) | ||

500.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

600.0 °C | 541 J/(kg·K) Show Material materials with Specific heat capacity of 541 J/(kg·K) | ||

700.0 °C | 551 J/(kg·K) Show Material materials with Specific heat capacity of 551 J/(kg·K) | ||

800.0 °C | 559 J/(kg·K) Show Material materials with Specific heat capacity of 559 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 13.9 - 15 W/(m·K) Show Material materials with Thermal conductivity of 13.9 - 15 W/(m·K) | |

100.0 °C | 15.4 W/(m·K) Show Material materials with Thermal conductivity of 15.4 W/(m·K) | ||

200.0 °C | 17.2 W/(m·K) Show Material materials with Thermal conductivity of 17.2 W/(m·K) | ||

300.0 °C | 18.7 W/(m·K) Show Material materials with Thermal conductivity of 18.7 W/(m·K) | ||

400.0 °C | 20.2 W/(m·K) Show Material materials with Thermal conductivity of 20.2 W/(m·K) | ||

500.0 °C | 21.6 W/(m·K) Show Material materials with Thermal conductivity of 21.6 W/(m·K) | ||

600.0 °C | 23 W/(m·K) Show Material materials with Thermal conductivity of 23 W/(m·K) | ||

700.0 °C | 24.4 W/(m·K) Show Material materials with Thermal conductivity of 24.4 W/(m·K) | ||

800.0 °C | 25.8 W/(m·K) Show Material materials with Thermal conductivity of 25.8 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 3.7 mm²/s Show Material materials with Thermal diffusivity of 3.7 mm²/s | |

100.0 °C | 3.9 mm²/s Show Material materials with Thermal diffusivity of 3.9 mm²/s | ||

200.0 °C | 4.2 mm²/s Show Material materials with Thermal diffusivity of 4.2 mm²/s | ||

300.0 °C | 4.5 mm²/s Show Material materials with Thermal diffusivity of 4.5 mm²/s | ||

400.0 °C | 4.7 mm²/s Show Material materials with Thermal diffusivity of 4.7 mm²/s | ||

500.0 °C | 4.8 mm²/s Show Material materials with Thermal diffusivity of 4.8 mm²/s | ||

600.0 °C | 5 mm²/s Show Material materials with Thermal diffusivity of 5 mm²/s | ||

700.0 °C | 5.3 mm²/s Show Material materials with Thermal diffusivity of 5.3 mm²/s | ||

800.0 °C | 5.6 mm²/s Show Material materials with Thermal diffusivity of 5.6 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 7.3E-7 - 7.35E-7 Ω·m Show Material materials with Electrical resistivity of 7.3E-7 - 7.35E-7 Ω·m |

100.0 °C | 8E-7 Ω·m Show Material materials with Electrical resistivity of 8E-7 Ω·m | |

200.0 °C | 8.68E-7 Ω·m Show Material materials with Electrical resistivity of 8.68E-7 Ω·m | |

300.0 °C | 9.33E-7 Ω·m Show Material materials with Electrical resistivity of 9.33E-7 Ω·m | |

400.0 °C | 9.89E-7 Ω·m Show Material materials with Electrical resistivity of 9.89E-7 Ω·m | |

500.0 °C | 1.04E-6 Ω·m Show Material materials with Electrical resistivity of 1.04E-6 Ω·m | |

600.0 °C | 1.08E-6 Ω·m Show Material materials with Electrical resistivity of 1.08E-6 Ω·m | |

700.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

800.0 °C | 1.15E-6 Ω·m Show Material materials with Electrical resistivity of 1.15E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.03 % Show Material materials with Carbon of 0.03 % |

Chromium | 18 - 20 % Show Material materials with Chromium of 18 - 20 % |

Manganese | 2 % Show Material materials with Manganese of 2 % |

Nickel | 10 - 12 % Show Material materials with Nickel of 10 - 12 % |

Nitrogen | 0.1 - 0.11 % Show Material materials with Nitrogen of 0.1 - 0.11 % |

Phosphorus | 0.05 % Show Material materials with Phosphorus of 0.05 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |